**Soft Matter **

## PAPER

*This journal is © The Royal Society of Chemistry 2017 * *Soft Matter, 2017, 00, 1-3| ***1 **

*a _{Key Laboratory of Beijing City on Preparation and Processing of Novel Polymer }*

*Materials, State Key Laboratory of Organic-Inorganic Composites, Beijing *
*University of Chemical Technology, 100029 Beijing, China *

*E-mail: [email protected], [email protected]. *

*b _{ Hubei Collaborative Innovation Center for Advanced Organic Chemical Materials, }*

*Key Laboratory for the Green Preparation and Application of Functional Materials, *
*Ministry of Education, Hubei Key Laboratory of Polymer Materials, School of *
*Materials Science and Engineering, Hubei University, 430062 Wuhan, China *

*c _{CNR-SPIN, Via Cintia, 80126 Napoli, Italy }*

*d _{Dipartimento di Chimica, Materiali e Ingegneria Chimica ‘‘G. Natta’’, Politecnico}*

*di Milano, via L. Mancinelli 7, 20131 Milano, Italy *
Received 00th January 20xx,

Accepted 00th January 20xx
DOI: 10.1039/x0xx00000x
**www.rsc.org/ **

**Effects of Chemically Heterogeneous Nanoparticles on Polymer **

**Dynamics: Insights from Molecular Dynamics Simulations **

**Zijian Zheng,ab _{ Fanzhu Li,}a_{ Jun Liu,}* a_{ Raffaele Pastore,}c,d_{ Guido Raos,}d_{ Youping Wu,}a_{ Liqun }**

**Zhang * a**

The dispersion of solid nanoparticles within polymeric materials is widely used to enhance their performance.
Many scientific and technological aspects of the resulting polymer nanocomposites have been studied, but the
role of the structural and chemical heterogeneity of nanoparticles has just started to be appreciated. For
example, simulations of polymer films on planar heterogeneous surfaces revealed unexpected, non-monotonic
activation energy to diffusion on varying the surface composition. Motivated by these intriguing results, here
we simulate via molecular dynamics a different, fully three-dimensional system, in which heterogeneous
nanoparticles are incorporated in a polymer melt. The nanoparticles are roughly spherical assemblies of
*strongly and weakly attractive sites, in fraction f and 1-f, respectively. We show that polymer diffusion is *
*still characterized by non-monotonic dependence of the activation energy on f. The comparison with *
the case of homogeneous nanoparticles clarifies that the effect of the heterogeneity increases on
approaching the polymer glass transition.

**I. Introduction **

The introduction of nanoparticles (NPs) into polymer matrices
is an effective strategy to fabricate high performance polymer
nanocomposites (PNCs)1-3_{. A fundamental understanding of }

their composition-structure-properties relationship will facilitate the further development of materials with desired

properties4_{. One key lesson is that it is crucial to disperse the }

nanoparticles well in the polymer matrix in order to produce
high performance composites5_{. This can be achieved by }

compatibilizing them, for example by coating the nanoparticles
or grafting them with the polymer6-8_{. }

The interface between polymers and nanoparticles is also a
very important element. In the nanometer-size interstices
between the nanoparticles, the polymer chains become severely
restricted and may deviate substantially from their bulk
behavior9_{. Thus, the polymer interfaces which are formed near }

solid surfaces and nanoparticles have received wide
consideration from both the academic and industrial
communities10-14_{. One of the earliest studies is the one by }

Tsagaropoulos and Eisenberg15_{, who observed that several }

polymer properties such as viscosity, diffusion coefficient, and the T2 relaxation time in NMR measurements were drastically

altered by silica nanoparticles and attributed this effect to a
drastic slowing down of the chains in the interfacial region.
Later on, Torkelson and coworkers16, 17_{ studied the relaxation of }

thin polymer films on silica surfaces, as a model for polymer-silica nanocomposites. Using fluorescent probes to monitor the dynamics of the polymer matrix, they demonstrated that chains next to the surface were nearly completely arrested (at temperatures above the bulk Tg), but the slowing down in the

relaxation dynamics could be felt up to 100 nm away from it.
Even a small concentration of nanoparticles can slow down
significantly the polymer diffusion within a PNC, due to a
combination of the reduced polymer relaxation and the entropic
barriers created by the excluded volume of the NPs18_{. NP }

induced enhancement of the polymer relaxation rate has been
also observed for particular physical situations, including
systems formed by entangled polymers and NPs smaller than
the entanglement mesh size19_{. }** **

Many useful insights have been obtained by theoretical
analyses and molecular dynamics (MD) or Monte Carlo
simulations, alongside the traditional experimental methods
20-22_{. Smith et al.}23_{ introduced some structural roughness in the }

coarse-grained modelling of NPs. Starr et al.24_{ found a mobility }

gradient for coarse-grained polymer chains approaching the
nanoparticle surfaces, both for repulsive and attractive
polymer/nanoparticle interactions. Li et al.25 _{explored the }

dynamics of long polymer chains filled with spherical NPs.
Through a primitive path analysis, they showed that the chains
become significantly disentangled on increasing the NP volume
fraction, but “NP entanglements” become significant above a
critical volume fraction. More recently, Hagita et al.26_{ have }

performed large-scale MD simulations of related cross-linked
models, to describe the mechanical deformation of rubbery
nanocomposites with different degrees of particle aggregation.
At the atomistic level of description, Ndoro et al.27_{ simulated a }

composite consisting of ungrafted and grafted spherical silica

nanoparticles embedded in a melt of 20-monomer atactic
polystyrene chains. These showed that the nanoparticles modify
the polymer structure in its neighborhood, and these changes
increase with the higher grafting densities and larger particle
diameters. De Nicola et al.28_{ used the results of molecular }

simulation as a guide for the preparation of improved
*polymer-NP composites, exploiting an in situ polymerization of *
macromonomers.

Most of the previous simulations, especially those based
on coarse-grained models, employed completely smooth or
structured NPs with chemically uniform surfaces. However the
most common fillers, namely silica29_{ and especially carbon }

black30, 31_{ for applications involving mechanical reinforcement, }

have heterogeneous surfaces exposing a range of functional
groups and adsorption sites (e.g., both hydrophobic and
hydrophilic, hydrogen-bonding groups). Note that the slight
roughness of an atomically structured surface has already a
very significant effect on the polymer dynamics, in comparison
to the idealized situation with a perfectly smooth surface32_{. An }

even greater effect can be expected from the introduction of
some chemical heterogeneity in the surfaces and/or the
polymer. In fact, there is ample evidence that this sort of
‘‘quenched’’ disorder plays an important role in many aspects
of polymer behavior33_{. Recent insights came from MD }

simulations of thin polymer films adsorbed on structurally and chemically heterogeneous surfaces. These latter are composed by randomly assembling on a planar square lattice two type of beads, strongly (S) and weakly (W) attractive, in variable percentage. In such a quasi-2D model, the dynamic slowdown of polymers was found to depend non-monotonically on the surface composition: the activation energy to diffusion and the inverse glass transition temperature do not attain a maximum for 100% of strong sites, but at a smaller value, about 75%, which originates as a compromise between the maximum global attraction and the maximum configurational disorder at the random percolation (50%) of strong sites. In addition, new dynamical features, which are not observed on a smooth surface, become more and more apparent on increasing the

**Journal Name ** **ARTICLE **

*This journal is © The Royal Society of Chemistry 2017 * *Soft Matter,* 2017, **00, 1-3| 3 **

surface heterogeneity. These include temporary subdiffusive regimes followed by “Fickian yet not Gaussian diffusion” as well as stretched exponential relaxation of the Rouse Normal Modes autocorrelation functions.

In this paper, we aim at understanding whether these
intriguing benchmarks are also relevant to fully
three-dimensional polymer nanocomposite, where NPs are finely
dispersed within the polymer melts. This is not a trivial
question, since the different dimensionality, the coexistence of
adsorbed and non-adsorbed polymers as well as the presence of
NP induced steric interactions make this physical situation
markedly distinct from that described in Ref.s34,35_{. We }

investigate this issue by introducing a coarse-grained model of
polymer melt embedding a number of heterogeneous NPs. Each
NP consists in a roughly spherical assembly of W and S sites.
Performing extensive MD simulations, we investigate the
polymer dynamics at different temperatures and variable NP
composition. We find that, in spite of the difference between
the two physical situations, some dynamical signatures found in
Refs.34,35 _{survive in this system, suggesting the existence of a }

common underlying physical mechanism. In addition, we clarify to what extent the heterogeneous nature of the NPs modifies the polymer dynamics compared to the homogeneous case, showing that relatively small differences at high temperature may result in dramatic change close the polymer glass transition.

**II. Simulation model and method **

In our coarse-grained model, the heterogeneous NPs are roughly spherical and are composed by two types of randomly distributed beads, which may be either of the weak (W) or the strong (S) type, the only difference being the interaction energy with polymers. A snapshot is shown in Fig. 1. Briefly, we first generate one NP, formed by N=128 beads, Ne=74 of which are

exposed, and replicate such a prototype within the simulation box until the desired number of NPs is reached. At this stage, we randomly assign the interaction energy (i. e. the type) to

each bead with probability f and 1-f for strong (S) and weak
(W) interactions, respectively.36_{ }

The simulation box contains 30 nanoparticles, which corresponds to a volume fraction of NPs ϕ=0.253 (estimated from the total numbers of NP-type and polymer-type beads). During the MD simulations, the NPs are modelled as perfectly rigid bodies, with only three translational and three rotational degrees of freedom.

Fig. 1 The snapshots of nanoparticle, polymer chain and the corresponding nanocomposite. Within the NPs, the blue spheres represent the S sites and the red spheres represent the W sites.

The polymer chains are fully flexible and are represented
by a generic bead-spring model. Overall, each polymer chain
contains 32 beads. Given the relatively short length of the
polymer chains, entanglement effects play a minor role on the
system dynamics. Roughly, each bond of the coarse-grained
model would correspond to 3-6 covalent bonds along the
backbone of a chemically realistic chain. However, since we
are not interested in a specific polymer, it is unnecessary to
attempt a precise mapping. We adopt a “reduced” set of units,
*whereby the mass m and diameter σ of each bead-which are *
identical for the polymer and the NPs-are effectively equal to
unity. The non-bonded interactions between all the beads are
modeled by truncated and shifted Lennard-Jones (LJ)
potentials:
𝑈𝑈(𝑟𝑟) = �4𝜀𝜀 ��𝜎𝜎𝑟𝑟�
12
− �𝜎𝜎_{𝑟𝑟�}6� + 𝐶𝐶 𝑟𝑟 < 𝑟𝑟𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐
0 𝑟𝑟 ≥ 𝑟𝑟𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐
(1)
*where C is a constant which guarantees that the potential *
*energy is continuous at r=rcutoff*, and *ε is the energy scale of the *

model. While the effective diameter σ is the same for all beads,
both the interaction energy and the cutoff distance depend on
the combination of bead types. The interaction strength
between the polymer beads (P) and the S sites is twice that of
the other pairs. Thus *ɛ*PP =*ɛ*PW=*ɛ and ɛ*PS=2*ɛ. All the *

*polymer-NP interactions are truncated at a cutoff distance of r*PW*=r*PS

=2.5*σ, whereas the polymer–polymer interactions are truncated *
*at r*PP = 21/6*σ to produce a purely repulsive potential. Also the *

interaction between the beads belonging to different NP is
modelled with *ɛ*NN=*ɛ (where N=W or S) and the cutoff *

*r*NN=21/6*σ, so as to promote their dispersion within the polymer *

matrix. By doing so, we aim at modelling the physical situation of finely dispersed NPs within the polymer melts, which can be achieved in different experimental setups, such as samples freshly rejuvenated at high shear rate. In systems of this kind, the typical separation distance between NPs is large enough to make van der Waals interactions negligible.

The interaction between bonded beads within a polymer is modeled by adding a finite extensible nonlinear elastic (FENE) potential to their LJ interaction:

𝑈𝑈𝐹𝐹𝐹𝐹𝐹𝐹𝐹𝐹= −0.5𝑘𝑘𝑅𝑅02𝑙𝑙𝑙𝑙 �1 − �_{𝑅𝑅}𝑟𝑟
0�

2

� (2)
*where k=30ε/σ2*_{ is the force constant and R}

0=1.3*σ is the *

maximum extensibility of the bonds. The finite extensibility of
the bonds avoids chain crossing events without introducing
high-frequency bond vibrations, which would be produced by
very stiff harmonic bonds. The relatively short maximum bond
length enhances the polymer’s resistance to ordering and
crystallization, by increasing the mismatch between bonded and
non-bonded nearest-neighbor distances (the actual equilibrium
bond length, resulting from the balance between LJ and FENE
interactions, is about 0.8*σ)*37_{. The reduced number density of }

the monomer was fixed at *ρ* =1.00, which corresponds to that *
of a dense melt. This is also roughly equal to the density inside
the NPs. Units are reduced so that *σ=m=ɛ=kB=1, where kB* is the

Boltzmann’s constant.

We have performed NVT molecular dynamics

simulations, using a Nose-Hoover thermostat and
velocity-Verlet algorithm to integrate the equations of motion. Periodic
boundary conditions are applied to all three directions. The
average MD run consists of 109_{ time steps. All the simulations }

have been carried out with a large scale atomic/molecular
massively parallel simulator (LAMMPS), developed by the
Sandia National Laboratories38_{. Further simulation details can }

be found in our previous work39,40_{. }

**III. Results **

**3.1 Translational dynamics **

We start by investigating the effect of heterogeneous NPs on
the translational dynamics of the whole polymer chains. To this
aim, Fig. 2 shows the time dependence of the mean square
displacements (MSDs) of the polymer center of mass, for
*different NP composition, f, and temperature, T**_{. The mobility }

of the polymer chains becomes small on lowering the temperature and for large values of f and display an increasingly long lasting subdiffusive behaviuour. However, even for the slowest system, the diffusive regime is restored within the timescale of our simulations,

〈�𝑟𝑟𝑐𝑐𝑐𝑐(𝑡𝑡)−𝑟𝑟𝑐𝑐𝑐𝑐(0)�2〉 = 6 𝐷𝐷 𝑡𝑡 (3)

*allowing to estimate the chain diffusion coefficient, D, a long *
time fit to the MSD data. The diffusion coefficient so measured
are listed in Table 1 and plotted in Fig. 3a shows as a function
of temperature and at different values of f. This figure clarifies
that the data can be properly fitted using an Arrhenius
functional law:

𝑙𝑙𝑙𝑙(𝐷𝐷) = 𝑙𝑙𝑙𝑙(𝐷𝐷0) − 𝐸𝐸𝑎𝑎⁄ . (4)𝑇𝑇∗

*The values of the activation energies (Ea*) obtained from these

fits are plotted in Figure 3b as a function of the NP composition, f, and listed in the last line of Table 1.

**Journal Name ** **ARTICLE **

*This journal is © The Royal Society of Chemistry 2017 * *Soft Matter,* 2017, **00, 1-3| 5 **

*Table 1. Polymer Diffusion Coefficients for Each Reduced Temperature (T*) and Surface Composition (f).The last row gives the *
*activation energies at different Surface Composition (f ). *

*T*/f * Neat 0.00 0.25 0.50 0.75 1.00
0.7 0.0019 _{4.84x10}-5 _{2.98x10}-5 _{1.62x10}-5 _{1.22x10}-5 _{1.15x10}-5
0.8 0.0021 _{7.63x10}-5 _{4.25x10}-5 _{3.54x10}-5 _{2.23x10}-5 _{1.93x10}-5
0.9 0.0023 _{1.11x10}-4 _{6.99x10}-5 _{4.89x10}-5 _{3.91x10}-5 _{2.94x10}-5
1.0 0.0026 _{1.48x10}-4 _{1.05x10}-4 _{7.31x10}-5 _{5.66x10}-5 _{4.37x10}-5
1.1 0.0027 _{1.88x10}-4 _{1.26x10}-4 _{1.02x10}-4 _{8.06x10}-5 _{6.41x10}-5
1.2 0.0030 _{2.08x10}-4 _{1.65x10}-4 _{1.32x10}-4 _{1.08x10}-4 _{8.95x10}-5
*Ea * 0.71±0.01 2.52±0.05 2.96±0.03 3.43±0.02 3.67±0.03 3.42±0.02

*Fig. 2 Mean square displacement as a function of time, for T* = *
1.2, 1.1, 1.0, 0.9, 0.8, and 0.7 from top to bottom. Different
*panels report different values of f, as indicated. Dashed lines are *
guides to the eye of slope 1.

Overall, the order of magnitude of the activation energy is
compatible with the results of previous work investigating
different polymer nanocomposite systems35_{. For the neat }

*polymer system, Ea* is due to crowding and excluded volume

effect, and therefore has an entropic origin. The presence of

NPs introduces attractive interaction and increases the
crowding effect. This results in significantly higher activation
*energy, even for f=0. In addition Fig. 3(b) shows that Ea as a *

*function f in Fig. 3(b) is maximal around f=0.75. This *
non-monotonic behaviour is intriguing, as the largest activation
energy to diffusion does not correspond to the situation where
the strength of the interaction is overall the largest, f=1, but to a
lower value of f. As previously mentioned, a similar result
emerged from the simulations of polymer films adsorbed on
heterogeneous planar surfaces of Ref.s34,35_{. In that case, the }

*value f=0.75 was interpreted as the compromise between the *
*largest overall interaction energy (f=1) and the maximum *
structural disorder, attained at the random percolation transition
*of strong sites (occurring around f=0.5, in two dimensions). *
This scenario was validated by an analysis of the surface
induced energy landscape, as probed by horizontally sliding a
single bead along the surface at very low temperature. The
average value of the energy barriers linearly increases between
*f=0 and f=1, whereas the standard deviation is the largest for *
*the most disordered substrate f=0.5. Finally, the most *

significant descriptor of the dynamics are the tails of energy
*barrier distributions that are indeed the largest at f=0.75. *
Considering the similar behaviour found in the present model,
we speculate that the shape of the energy landscape and its
implications are also similar.

Fig. 3 Arrhenius plots of the chain diffusion coefficients (a) and plot illustrating the surface dependence of the activation energies (b).

**3.2 Rouse mode analysis **

The polymer chain dynamics can be further characterized by
investigating their conformational relaxation dynamics, which
is commonly characterized through the autocorrelation
functions 𝐶𝐶_{𝑝𝑝}(𝑡𝑡) = 〈𝑄𝑄_{𝑝𝑝}(0) ∙ 𝑄𝑄_{𝑝𝑝}(𝑡𝑡)〉 of the Rouse Normal Modes
(RNMs):
𝑄𝑄𝑝𝑝(𝑡𝑡) =_{𝑁𝑁 � 𝑟𝑟}1 𝑗𝑗(𝑡𝑡) 𝑐𝑐𝑐𝑐𝑐𝑐 �
�𝑗𝑗 −1_{2}� 𝑝𝑝𝑝𝑝
𝑁𝑁 � (5)
𝐹𝐹
𝑗𝑗=1

where 𝑟𝑟_{𝑗𝑗}*(𝑡𝑡) is the position of monomer j at time t, and p=1, *
*2, ..., N-1 is the mode index. Each mode p is associated with a *
typical length-scale, as it describes the collective motion of
*chain sections containing the N/p beads. Note that the polymer *
center-of-mass, which is relevant to the translational diffusion

*described previously, formally corresponds to the mode p=0. In *
*the following, we focus on the system with f=0.50. *

Fig. 4(a) shows 𝐶𝐶_{𝑝𝑝}*(𝑡𝑡) for different values of p at *
*temperature T*=1.0. Their decay becomes significantly faster *
*with increasing p, as the mode describes more localized *
motions. The decay of the autocorrelation functions appear to
be not consistent with a simple exponential, as predicted by the
Rouse model, being , instead, well described by a stretched
exponential, or Kohlrausch-Williams-Watts (KWW) function:

𝐶𝐶𝑝𝑝(𝑡𝑡) ≃ exp �−�𝑡𝑡 𝜏𝜏⁄ �𝑝𝑝𝑠𝑠 𝛽𝛽� (6)

This behaviour has been also reported in simulations of
polymer matrix embedding polymer grafted nanoparticles41_{ and }

is generally known to be a common hallmark of glassiness and
an indirect signature of the emergence of dynamic
heterogeneities.42_{ It is worth noticing that a crossover from }

stretched (*β<1) to compressed (β>1) exponential has been also *
observed in soft glassy materials, such as colloidal glasses43-46_{, }

gels47_{ and other amorphous solids}48_{, its origin being currently a }

very debated issue. We extract the parameters *β and 𝜏𝜏*_{𝑝𝑝}𝑠𝑠 from
KWW fits to the data of Fig.4a. In addition, we directly
measure the relaxation time using the standard relation,
𝐶𝐶𝑝𝑝�𝜏𝜏𝑝𝑝� = 1/𝑒𝑒 and found a very good agreement with the

estimation obtained from fits (see, for example, Fig. 5b)
Fig. 4(b) shows that *β decreases slightly on lowering the *
temperature but much more clearly on increasing the mode
*index, p, indicating that the relaxation of the chains tends to *
broaden on the local scale. A qualitatively similar effect was

*This journal is © The Royal Society of Chemistry 2017 * *Soft Matter, 2017, ***00, 1-3 | 7 **
Fig. 4 (a) RNM autocorrelation function 𝐶𝐶_{𝑝𝑝}*(𝑡𝑡) at f=0.50, T*=1.0 and p=1, 2, . . . , 5, from right to left. The open square represents *
*the KWW fit at different p. (b) Exponent *𝛽𝛽_{𝑝𝑝} and (c) the relaxation time (𝜏𝜏_{𝑝𝑝}, where 𝐶𝐶_{𝑝𝑝}�𝜏𝜏_{𝑝𝑝}�=1/e) corresponding to the first 5 modes
of polymer chains with different temperatures.

Fig. 5 (a) RNM autocorrelation function 𝐶𝐶_{𝑝𝑝}*(𝑡𝑡) for p=1 and T*=0.8, 0.9,..., 1.2, for heterogeneous NPs with f=0.5. The open square *
represents the KWW fit at different temperatures. (b) The data of panel (a) plotted in linear-log scale. (c) Fitted 𝜏𝜏_{1}𝑠𝑠 and
measured 𝜏𝜏_{1}*relaxation times as a function of 1/T*. *

also observed in model nanocomposites with homogeneous,
purely repulsive NPs by Li et al.49_{. However, at volume }

fractions comparable to ours, their stretching exponents for the
first five modes are in the 0.7-0.9 range, i.e. much closer to
unity than ours. Fig. 4(c) illustrates the dependence of the
relaxation times (𝜏𝜏_{𝑝𝑝}*) on the mode index p. We point out that at *
high temperature, T*=1.2, the relaxation time, 𝜏𝜏_{𝑝𝑝}= 𝑝𝑝−2.27±0.01,
deviates somewhat from the Rouse scaling law (𝜏𝜏_{𝑝𝑝}∝ (𝑁𝑁/𝑝𝑝)2,
*for p<<N), and the deviation becomes even more significant at *
the low temperature, T*=0.8, as we find 𝜏𝜏_{𝑝𝑝}= 𝑝𝑝−2.44±0.02.

Finally, we consider the effect of the temperature on the
autocorrelation functions 𝐶𝐶_{𝑝𝑝}(𝑡𝑡). Fig. 5(a) shows the behavior of
*the mode with p=1. Decreasing temperature decreases from 1.2 *
to 0.8, the decay becomes slower and slower but is always
properly fitted by KWW functions, allowing to measure the
parameters 𝛽𝛽_{𝑝𝑝} and 𝜏𝜏_{𝑝𝑝}𝑠𝑠* as a function of T*, as shown in Fig. 4(b). *
Figure 5(b) clarifies that the relaxation times 𝜏𝜏_{1}𝑠𝑠 and 𝜏𝜏_{1} as a
function of the temperature keeps on being consistent with an
Arrhenius behaviour: 𝑙𝑙𝑙𝑙(𝜏𝜏_{1}) = 3.65 ×1

𝑇𝑇∗+ 5.72, the resulting

activation energy being slightly larger than the one presented earlier for the translational diffusion.

In order to highlight the effect of the nanoparticle heterogeneities on the polymer chain relaxation, we compare

the result of Fig. 4 and 5 to an homogeneous system with
*ɛ*PW=*ɛ*PS=1.5*ɛ≡ɛnp*. This corresponds to a situation with

chemically homogeneous nanoparticles, which have, the same
*average polymer-particle interactions as the system with f=0.50. *
The results, illustrated in Fig. 6 and 7, highlight a number of
differences emerging with respect to the heterogenous case. For
example, deviatons from the Rouse model appears to be
weaker, especially concerning the relation between 𝜏𝜏_{𝑝𝑝}* and p In *
addition, the stretching exponent of the KWW decreases
significantly at low temperatures and increases significantly at
*high p, as shown in Fig. 6(d). The very good agreement *
between 𝜏𝜏_{1}𝑠𝑠 and 𝜏𝜏_{1} is also confirmed (Fig. 7). Finally, the
activation energy is slightly lower than in the heterogeneous
system:𝑙𝑙𝑙𝑙�𝜏𝜏_{𝑝𝑝}� = 3.58 × 1

𝑇𝑇∗+ 5.72 . Overall, this implies that

polymer relaxation is 5-10% faster than in the heterogeneous system, for the same average polymer-NP interaction strength. The difference increases on lowering the temperature.

Fig. 6 For the homogeneous system with *εnp*=1.5*ɛ: (a) RNM *

*autocorrelation function Cp(t) at, T*=1.0 and p=1, 2, . . . , 5, *

from right to left. (b) RNM autocorrelation function 𝐶𝐶_{𝑝𝑝}(𝑡𝑡) for
*p=1 and T*=0.8, 0.9, . . ., 1.2, from right to left. (c) The *
relaxation time (𝜏𝜏_{𝑝𝑝}) and (d) exponent 𝛽𝛽_{𝑝𝑝} for the first 5 modes of
polymer chains at different temperatures.

Fig. 7 Fitted 𝜏𝜏_{1}𝑠𝑠 and measured 𝜏𝜏_{1}relaxation time (𝐶𝐶_{𝑝𝑝}�𝜏𝜏_{𝑝𝑝}�=1/e)
*as a function of 1/T*. The nanocomposite filled with *
homogeneous nanoparticles. Note that this system have the
same average polymer-particle interactions as the system with
*f=0.50. *

**3.3 Structural relaxation **

In this section, we complement the previous analysis, based
on the center of mass dynamics, by investigating the segmental
dynamics. In particular, we compute the intermediate self
scattering function (ISSF), 𝜙𝜙_{𝑞𝑞}𝑠𝑠(𝑡𝑡). For an isotropic system:

𝜙𝜙𝑞𝑞𝑠𝑠_{(𝑡𝑡)}
=_{𝑀𝑀 �}1 〈𝑒𝑒𝑒𝑒𝑝𝑝(𝑖𝑖𝒒𝒒 ∙ [𝒓𝒓𝑐𝑐(𝑡𝑡) − 𝒓𝒓𝑐𝑐(0)])〉
𝑀𝑀
𝑐𝑐=1
= _{𝑀𝑀 �}1 〈𝑐𝑐𝑖𝑖𝑙𝑙�𝑞𝑞∆𝑟𝑟𝑐𝑐(𝑡𝑡)�
𝑟𝑟𝑐𝑐(𝑡𝑡) 〉
𝑀𝑀
𝑐𝑐=1
(6)

*where M is the total number of scattering centers in the *
polymer matrix, |𝑟𝑟_{𝑐𝑐}(𝑡𝑡) − 𝑟𝑟_{𝑐𝑐}(0)| = ∆𝑟𝑟_{𝑐𝑐}(𝑡𝑡) is the displacement of

*scattering center m after time t, and the wave-vector q=2π/λ, *
probes the dynamics at the length scale *λ. Similarly to a *
previous work by some of us50_{, we fix q=6.9 to probe the }

dynamics at segment length scale, i.e. the length scale relevant to the structural relaxation.

Fig. 8 ISSF, 𝜙𝜙_{𝑞𝑞}𝑠𝑠(𝑡𝑡), for the system filled with heterogeneous
nanoparticles at different temperatures T*=0.7, 0.8, 0.9, 1.0, 1.1
*and 1.2 for different f. *

Figure 10 shows the self intermediate scattering function
*for the heterogeneous case at different values of f. Similarly to *
what done for the RNM autocorrelation function, we measure
the structural relaxation time, τ_{ℎ𝑒𝑒𝑐𝑐}, from the standard relation,
𝜙𝜙𝑞𝑞𝑠𝑠(τℎ𝑒𝑒𝑐𝑐) = 𝑒𝑒−1. Fig. 9 shows the temperature dependence τ_{ℎ𝑒𝑒𝑐𝑐}
at different value of f. Once again, data are consistent with an
Arrhenius behaviour, but the activation energy monotonically
*increases with increasing f, differently from the diffusion *
constant of the chain center of mass. This difference can be
rationalized considering that the segment length scale is too

**Journal Name ** **ARTICLE **

*This journal is © The Royal Society of Chemistry 2017 * *Soft Matter,* 2017, **00, 1-3| 9 **

small for probing the presence of disorder in the spatial distribution of W and S sites, and, therefore, the dynamics on that length is controlled by the interaction strength only.

*Fig. 9 Structural relaxation time as a function of 1/T* for *
*different f. *

In order to further compare the effects of the heterogeneous
and homogeneous nanoparticles on the polymer relaxation, Fig.
10 and Fig. 11 show 𝜙𝜙_{𝑞𝑞}𝑠𝑠(𝑡𝑡) and the structural relaxation time for
*the heterogeneous case at f=0.5 and its homogeneous *
counterpart (*ɛnp* =1.5), respectively. Panel b of Fig.11 clarifies

that the structural relaxation time of the homogeneous system, τℎ𝑐𝑐𝑐𝑐𝑐𝑐 , also increases on lowering the temperature with an

Arrhenius fashion. In particular, we find that ln(τ_{het}) =
2.10 ×_{T}1∗− 1.99 and ln(τhomo) = 1.92 ×

1

T∗− 1.80, with the

associated activation energies resulting lower than those at the chain length scale. However, in both relative and absolute terms, the difference between the two activation energies increases on going from the chain length scale (+2%) for the heterogeneous nanoparticles) to the segment length scale (+9%). This is reasonable, considering that a long chain will always mediate over many energetically different situations. Overall, it appears clearly that, in the investigated temperature range, the difference between the homogeneous and the heterogeneous case is not dramatic. However, such difference is expected to become larger and larger on decreasing the temperature. For example, at the lowest temperature investigated in this paper, T=0.7, we observe τhet/τhomo =1.09

that might appear a quite small difference. Conversely, at T=0.3 (a temperature that cannot be achieved in simulations but is fully accessible in experiments29) τ

het/τhomo =1.5, as can be

extrapolated by the Arrhenius behaviour reported in fig 8b and 9b. Accordingly, the structural relaxation time and, therefore, the zero-shear viscosity of the heterogeneous systems are expected to be 50% larger than those of the homogeneous system.

Fig. 10 (a) ISSF 𝜙𝜙_{𝑞𝑞}𝑠𝑠(𝑡𝑡) for the system filled with heterogeneous
nanoparticles at different temperatures T*=0.7, 0.8, 0.9, 1.0, 1.1
and 1.2. (b) Fitted relaxation times (C_{p}�τ_{p}�=1/e) as a function
*of 1/T*. *

Fig. 11 (a) ISSF 𝜙𝜙_{𝑞𝑞}𝑠𝑠(𝑡𝑡) for the system filled with homogeneous
nanoparticles at different temperatures T*=0.7, 0.8, 0.9, 1.0, 1.1
*and 1.2. (b) Structural relaxation time as a function of 1/T*. *

**IV. Conclusion **

We investigated via molecular dynamics simulations a coarse-grained model of polymer filled with chemically and structurally heterogeneous nanoparticles. The heterogeneities render the model more realistic and similar to widely adopted fillers, such as carbon black. One important implication arises from the investigation of the polymer chain center of mass diffusion: the unexpected non monotonic dependence of the activation energy on the NP composition do emerge similarly to Ref. 29 and 30, although the investigated models are markedly different and reflect two different physical situations. This finding suggests the existence of a robust underlying physical

mechanism based on the interplay of interaction strength and configurational disorder. Indeed, such a non-monotonic nature disappears when focusing on the segmental dynamics, since the related probe length is too small to be sensitive to disorder. A more general motivation of this work consists in understanding to what extent the presence of heterogeneous NPs modifies the system dynamics compared to the homogeneous case. In this respect, we clarified that relatively small differences observed at high temperature are the precursor of larger and larger changes on approaching the glass transition. This suggests that the effect of the heterogeneities may be strongly relevant for polymers forming glassy shells around nanoparticles.

**Acknowledgements **

This work is supported by the National Basic Research Program of China 2015CB654700(2015CB654704), the Foundation for Innovative Research Groups of the NSF of China (51221002), the National Natural Science Foundation of China (51333004 and 51403015). The cloud calculation platform of BUCT is also greatly appreciated.

**References **

(1) RamanathanT, A. A. Abdala, StankovichS, D. A. Dikin, M.
Herrera Alonso, R. D. Piner, D. H. Adamson, H. C. Schniepp,
ChenX, R. S. Ruoff, S. T. Nguyen, I. A. Aksay, R. K.
* Prud'Homme and L. C. Brinson, Nat. Nano., 2008, 3, 327-331. *
(2) Q. Chen, S. Gong, J. Moll, D. Zhao, S. K. Kumar and R. H.

**Colby, ACS Macro Lett., 2015, 4, 398-402.**(3) P. Akcora, H. Liu, S. K. Kumar, J. Moll, Y. Li, B. C.
Benicewicz, L. S. Schadler, D. Acehan, A. Z. Panagiotopoulos,
V. Pryamitsyn, V. Ganesan, J. Ilavsky, P. Thiyagarajan, R. H.
**Colby and J. F. Douglas, Nat. Mater., 2009, 8, 354. **

(4) J. Jancar, J. F. Douglas, F. W. Starr, S. K. Kumar, P.
Cassagnau, A. J. Lesser, S. S. Sternstein and M. J. Buehler,
**Polymer, 2010, 51, 3321-3343. **

*(5) A. C. Balazs, T. Emrick and T. P. Russell, Science, 2006, *

**314, 1107. **

(6) L. Wang, K. G. Neoh, E. T. Kang, B. Shuter and S.-C.
**Wang, Adv. Funct. Mater., 2009, 19, 2615-2622. **

(7) S. Kango, S. Kalia, A. Celli, J. Njuguna, Y. Habibi and R.
**Kumar, Prog. Polym. Sci., 2013, 38, 1232-1261. **

(8) T. Mondal, R. Ashkar, P. Butler, A. K. Bhowmick and R.
**Krishnamoorti, ACS Macro Lett., 2016, 5, 278-282. **

(9) E. K. Lin, R. Kolb, S. K. Satija and W. l. Wu,
**Macromolecules, 1999, 32, 3753-3757. **

*(10) Z. Wang, Q. Lv, S. Chen, C. Li, S. Sun and S. Hu, ACS. *
**Appl. Mater. Iner., 2016, 8, 7499-7508. **

(11) *G. Maurel, F. Goujon, B. Schnell and P. Malfreyt, J. Phys. *
**Chem. C, 2015, 119, 4817-4826. **

(12) D. N. Voylov, A. P. Holt, B. Doughty, V. Bocharova, H.
M. Meyer, S. Cheng, H. Martin, M. Dadmun, A. Kisliuk and A.
**P. Sokolov, ACS Macro Lett., 2017, 6, 68-72. **

(13) A. Karatrantos, R. J. Composto, K. I. Winey and N.
**Clarke, N., J. Chem Phys., 2017, 146, 203331. **

* (14) J. J. Burgos-Mármol and A. Patti, Polymer, 2017, 113, *
92-104.

(15)* G. Tsagaropoulos and A. Eisenburg, Macromolecules, *
1995, 28, 396-398.

(16) R. D. Priestley, C. J. Ellison, L. J. Broadbelt and J. M.
**Torkelson, Science, 2005, 309, 456. **

* (17) C. J. Ellison and J. M. Torkelson, Nat. Mater., 2003, 2, *
695-700.

(18) C. C. Lin, S. Gam, J. S. Meth, N. Clarke, K. I. Winey and
* R. J. Composto, Macromolecules, 2013, 46, 4502-4509. *
(19) J. T. Kalathi, S. K. Kumar, M. Rubinstein and G. S. Grest,

**Soft matter, 2015, 11, 4123-4132.*** (20) V. Ganesan and A. Jayaraman, Soft Matter, 2014, 10, *
13-38.

(21)* J. Castillo-Tejas, S. Carro and O. Manero, ACS Macro *
**Lett., 2017, 6, 190-193. **

(22) J. Hager, R. Hentschke, N. W. Hojdis and H. A.
**Karimi-Varzaneh, Macromolecules, 2015, 48, 9039-9049. **

*(23) G. D. Smith, D. Bedrov, L. Li and O. Byutner, J. Chem *
*Phys., 117, 2002 9478-9489. *

(24) F. W. Starr, T. B. Schrøder and S. C. Glotzer,
**Macromolecules, 2002, 35, 4481-4492. **

(25)* Y. Li, M. Kröger and W. K. Liu, Phys. Rev. Lett., 2012, *

**109, 118001. **

*(26) K. Hagita, H. Morita, M. Doi, H. Takano, Macromolecules *
**2016, 49, 1972-1983. **

(27) T. V. M. Ndoro, E. Voyiatzis, A. Ghanbari, D. N.
Theodorou, M. C. Böhm and F. Müller-Plathe,
**Macromolecules, 2011, 44, 2316-2327. **

(28) A. De Nicola, R. Avolio, F. Della Monica, G. Gentile, M.
*Cocca, C. Capacchione, M. E. Errico and G. Milano, RSC Adv., *
**2015, 5, 71336-71340. **

(29) *G. E. Maciel and D. W. Sindorf, J. Am. Chem. Soc., 1980, *

**102, 7606-7607. **

(30) M. L. Studebaker, E. W. D. Huffman, A. C. Wolfe and L.
**G. Nabors, Ind. Eng. Chem., 1956, 48, 162-166. **

**(31) T. A. Vilgis, Polymer, 2005, 46, 4223-4229. **

(32)* G. D. Smith, D. Bedrov and O. Borodin, Phys. Rev. Lett., *
**2003, 90, 226103. **

(33) *A. Baumgärtner and M. Muthukumar, M. Adv. Chem. *
*Phys., 1996, 94,625-708 *

**(34) R. Pastore and G. Raos, Soft Matter, 2015, 11, 8083-8091. *** (35) G. Raos and J. Idé, ACS Macro Lett., 2014, 3, 721-726. *
(36) Thus, both the total and the exposed number of S beads of
each NP may fluctuate according to a binomial distribution and

**Journal Name ** **ARTICLE **

*This journal is © The Royal Society of Chemistry 2017 * *Soft Matter,* 2017, **00, 1-3| 11 **

no spatial correlations exists among beads of the same or different type, apart from the random ones. In particular, the number of S exposed beads has mean value <Nes>=Ne f and

standard deviation, ΔNes=[Ne f (1-f)]1/2, with a maximum value

ΔNes=4.3 at f=0.5. While such a fluctuation is too small to

affect the dynamics of this model significantly, in general it
may be exploited as an additional source of heterogeneity.
*(37) M. E. Mackura and D. S. Simmons, J. Polym. Sci. Pol. *
*Phys. 2014, 52, 134-140. *

(38)*S. Plimpton, J. Comput. Phys. 1995, 117, 1-19. *

(39) Z. Zijian, W. Zixuan, W. Lu, L. Jun, W. Youping and Z.
**Liqun, Nanotechnology, 2016, 27, 265704. **

(40) J. Liu, Y.-L. Lu, M. Tian, F. Li, J. Shen, Y. Gao and L.
**Zhang, Adv. Funct. Mater., 2013, 23, 1156-1163. **

* (41) G. D. Hattemer and G. Arya, Macromolecules, 2015, 48, *
1240-1255.

(42) L. Berthier, G. Biroli, J.-P. Bouchaud, L. Cipeletti, W. van
Saarloos, Dynamical Heterogeneities in Glasses, Colloids, and
Granular Media, Oxford University Press, Oxford, UK, 2011.
* (43) P. Ballesta, A. Duri and L. Cipelletti, Nat. Phys., 2008, 4, *
550–554.

*(44) R. Pastore, G. Pesce and M. Caggioni, Scientific Reports, *
**2017, 7, 43496. **

(45) R. Pastore, G. Pesce, A. Sasso and M. Pica Ciamarra,
**Colloid Surface A, 2017, 532, 87–96. **

(46) R. Angelini, E. Zaccarelli, F. A. D. M. Marques, M.
* Sztucki, A. Fluerasu and G. Ruocco, Nat. Commun., 2014, 5, *
4049.

(47) M. Bouzid, J. Colombo, L.V. Barbosa and E. Del Gado,
**Nat. Commun., 2017, 8, 15846. **

*(48) E. E. Ferrero, K. Martens and J.-L. Barrat, Phys. Rev. Lett., *
**2014, 113 ,248301. **

(49)* Y. Li, M. Kroger and W. K. Liu, Soft Matter, 2014, 10, *
1723-1737.

(50) *J. Liu, D. Cao, L. Zhang and W. Wang, Macromolecules, *
**2009, 42, 2831-2842. **